In metallurgy, the term phase is used to refer to a physically homogeneous state of matter, where the phase has a certain chemical composition, and a distinct type of atomic bonding and arrangement of elements. Within an alloy, two or more different phases can be present at the same time. The images below show the phases in aluminum-copper and iron-carbon alloys.
Each phase within an alloy has its own distinct physical, mechanical, electrical, and electrochemical properties. For example, in carbon steel, ferrite is a relatively soft phase and cementite is a hard, brittle phase. When they are present together, the strength of the alloy is much greater than for ferrite and the ductility is much better compared to cementite. Thus, an alloy with more than one phase can be considered to be a composite material.
The phases present in an alloy depend on the alloy composition and the thermal treatment to which the alloy has been exposed. Phase diagrams are graphical representations of the phases present in a particular alloy being held at a particular temperature. Phase diagrams can be used to predict the phase changes that have occurred in an alloy that has been exposed to a particular heat treatment process. This is important because the properties of a metal component depend on the phases present in the metal.
Phase diagrams are useful to metallurgists for selection of alloys with a specific composition and design and control of heat treatment procedures that will produce specific properties. They are also used to troubleshoot quality problems.
Iron-Carbon Phase Diagram
An example of a commonly used phase diagram is the iron-carbon phase diagram, which is used to understand the phases present in steel. The amount of carbon present in an iron-carbon alloy, in weight percent, is plotted on the x-axis and temperature is plotted on the y-axis. Each region, or phase field, within a phase diagram indicates the phase or phases present for a particular alloy composition and temperature. For the iron-carbon phase diagram, the phase fields of interest are the ferrite, cementite, austenite, ferrite + cementite, ferrite + austenite, and austenite + cementite phase fields.
The phase diagram indicates that an iron-carbon alloy with 0.5% carbon held at 900 °C will consist of austenite, and that the same alloy held at 650 °C will consist of ferrite and cementite. Furthermore, the diagram indicates that as an alloy with 0.78% carbon is slow cooled from 900 °C, it will transform to ferrite and cementite at about 727 °C.
Aluminum-Copper Phase Diagram
Another commonly used phase diagram is the aluminum-copper phase diagram, which is useful for understanding precipitation strengthening in Al-Cu alloys. The amount of copper present in an alloy is plotted on the x-axis. The phase fields of interest are the Al, θ, and Al+θ phase fields on the left hand side. For precipitation strengthening an Al-Cu alloy, this phase diagram indicates the minimum temperature to which an alloy must be heated to put all the copper in solution. This is indicated by the solvus line on the phase diagram. The maximum amount of copper that can contribute to precipitation strengthening is indicated by the maximum amount of copper (5.45 %) that can go into solid solution in the aluminum.
Phase diagrams indicate the relationship between the phases present, alloy composition, and temperature under conditions of slow heating or cooling. Slow heating or cooling allows the atoms within a metal to move around so that the alloy is at equilibrium. However, with many heat treatment processes, a metal is exposed to fast heating and cooling. Under these conditions it is possible to have phases missing or present compared to what is indicated by the phase diagram. Therefore, it is also important to understand the kinetics of phase transformations, i.e. the effects of temperature, time, cooling rate, and heating rate on phase changes within an alloy. This will be a topic of another article.
You can learn more about how to read and use phase diagrams in a few of our courses. Metallurgy of Steel and Metallurgy of Steel Heat Treating teach about the iron-carbon phase diagram. Metallurgy of Precipitation Strengthening teaches about the aluminum-copper phase diagram.
"A group of us took several courses (Principles of Metallurgy, Metallurgy of Steel, Corrosion of Metals) to become more knowledgeable about the science of metals to avoid problems. For me, the biggest impact of the training was on working with suppliers. I feel more confident asking questions and I now know the suppliers which know their stuff and which ones don’t. And it was great being able to get the training when it was convenient for me."Sam Bloodgood, VP Process Improvement, Hydraforce, Inc.
"I oversee several operations, including steel heat treating and laser welding. However, my background was in the construction materials industry. Principles of Metallurgy gave me the knowledge to have meaningful discussions with my engineers and be able to ask them better questions."Tom Parkman, Plant Manager, Simonds International.
“Principles of Metallurgy exceeded my expectations. The content was straightforward enough not to be burdensome, yet deep enough to provide a practical review of fundamental principles. I recommend this course to any engineer or technical person who has been out of school and working in industry for several years, but not necessarily having been focused on metallurgy.”Andy Jacobs, Staff Engineer, DePuy Orthopaedics, Inc.
“The Principles of Metallurgy course is broke up into convenient length modules that can be fit into the busiest schedule. The course is a good review for engineers who had a materials class ten or more years ago.”Paul Flury B/E Aerospace
“This is an excellent course (Metallurgy of Steel Heat Treating) for learning basic heat treating practices. The course introduces and covers a broad range of processes. I would recommend it for anyone in the steel business.”Jim Marks, Magellan Corporation
“This course has given me more confidence in my job and given me a better understanding of some of the heat treatments used in the business.”Mark Winter, Abbey Forged Products
Why Industrial Metallurgists?
- Practical, up-to-date content.
- Metallurgy expertise and 20+ years of experience.
- Courses designed for non-metallurgists.
- Training accessible from anywhere with internet access.
- Engaging content.
- Convenience. Learn when it suits your schedule.
- Avoid being overwhelmed with too much information at one time. Set your own pace.